macroporous methacrylated hyaluronic acid ... macroporous methacrylated hyaluronic acid cryogels of
Post on 19-Jun-2020
Embed Size (px)
Contents lists available at ScienceDirect
journal homepage: www.elsevier.com/locate/carbpol
Macroporous methacrylated hyaluronic acid cryogels of high mechanical strength and flow-dependent viscoelasticity
Burak Tavsanli, Oguz Okay⁎ Department of Chemistry, Istanbul Technical University, 34469 Maslak, Istanbul, Turkey
A R T I C L E I N F O
Keywords: Hyaluronic acid Cryogels Macroporous Viscoelasticity Mechanical properties
A B S T R A C T
We present here a new approach for the fabrication of macroporous hyaluronic acid (HA) cryogels with a tunable porous structure, flow-dependent viscoelasticity, and a high mechanical strength. They were synthesized from methacrylated HA in aqueous solutions at −18 °C by free-radical mechanism using in situ prepared poly(N, N- dimethylacrylamide) (PDMAA) as a spacer. Both the porosity and the average diameter of the pores decrease from 99 to 90% and from 150 to 90 μm, respectively, with increasing PDMAA content of the cryogels due to the simultaneous decrease in the amount of ice template during cryogelation. The cryogels also exhibit reversible strain-dependent apparent gel-to-sol transition due to the flowing-out and flowing-in water through the pores. This flow-dependent viscoelasticity is of great interest as it protects HA network from damage under large strain and hence acts as a self-defense mechanism.
Hyaluronic acid (HA), a significant component of the extracellular matrix, is a high-molecular weight natural polysaccharide with a large water holding capacity due to its polyelectrolyte nature (Fraser, Laurent, & Laurent, 1997). Although HA attracts significant interest over many years in soft tissue regeneration due to its excellent lu- bricating, self-healing, and biological functions (Chen & Abatangelo, 1999; Zamboni, Viera, Reis, Oliveira, & Collins, 2018), easy degrad- ability and weak mechanical behavior of HA limit its application areas (Collins & Birkinshaw, 2008; Valachova et al., 2016). To overcome these limitations, hydrogels based on native or chemically modified HA have been reported (Collins & Birkinshaw, 2008; Leach, Bivens, Patrick, & Schmidt, 2003; Prado, Weaver, & Love, 2011; Tavsanli, Can, & Okay, 2015). Several cross-linkers including ethylene glycol diglycidyl ether (EGDE), glutaraldehyde, and divinyl sulfone have been used in the preparation of HA hydrogels (Collins & Birkinshaw, 2007, 2013; Horkay, Hecht, & Geissler, 2006; Hwang et al., 2012; Kim et al., 2012; Segura et al., 2005; Tomihata & Ikada, 1977). Alternatively, HA was first modified to incorporate methacrylate groups to enable cross- linking, and then polymerized to form HA hydrogels (Ibrahim, Kothapalli, Kang, & Ramamurthi, 2011; Leach et al., 2003; Prado et al., 2011). It was shown that the hydrogels based on both native and me- thacrylated HA exhibit a good biocompatibility as well as a slow rate of degradation as compared to the native uncross-linked HA (Weng,
Gouldstone, Wu, & Chen, 2008). However, these hydrogels are gen- erally brittle in nature because of the lack of an effective energy dis- sipation in the covalently cross-linked HA network (Ahagon & Gent, 1975; Brown, 2007).
Recently, we have shown that an improvement in the mechanical properties of HA hydrogels could be achieved when silk fibroin is in- corporated into the HA network that forms β-sheet crystallites acting as physical cross-links (Tavsanli & Okay, 2019). Another strategy is double- or triple-networking of HA hydrogels with ductile network components based on poly(N,N-dimethylacrylamide) (PDMAA) (Tavsanli et al., 2015; Weng et al., 2008), a non-cytotoxic polymer for various applications interfacing with biological systems such as in medicine (Babic et al., 2009; Li et al., 2011; Wang, Yong, Deng, & Wu, 2018; de Queiroz, Castro, & Higa, 1997; Abraham, de Queiroz, & Roman, 2001). Although a mechanical property improvement in the resulting double- or triple-network HA hydrogels could be achieved, this multi-step synthetic procedure is lengthy and complicated.
Cryogelation is a simple and versatile technique for the fabrication of macroporous hydrogels, also called cryogels (Lozinsky & Okay, 2014; Lozinsky, 2002; Okay & Lozinsky, 2014). It is also more en- vironmentally friendly as compared to alternative techniques because water is generally used as the solvent, and there is no need to use or- ganic solvents as porogens. The principle of this technique is to carry out the cross-linking reactions of linear polymers in aqueous solutions below their freezing points. As water freezes, polymer chains rejected
https://doi.org/10.1016/j.carbpol.2019.115458 Received 6 September 2019; Received in revised form 26 September 2019; Accepted 7 October 2019
⁎ Corresponding author. E-mail address: firstname.lastname@example.org (O. Okay).
Carbohydrate Polymers 229 (2020) 115458
Available online 15 October 2019 0144-8617/ © 2019 Elsevier Ltd. All rights reserved.
http://www.sciencedirect.com/science/journal/01448617 https://www.elsevier.com/locate/carbpol https://doi.org/10.1016/j.carbpol.2019.115458 https://doi.org/10.1016/j.carbpol.2019.115458 mailto:email@example.com https://doi.org/10.1016/j.carbpol.2019.115458 http://crossmark.crossref.org/dialog/?doi=10.1016/j.carbpol.2019.115458&domain=pdf
from the ice and concentrated in the unfrozen regions result in the formation of a highly concentrated solution phase, called cryoconcen- tration. Thus, cryogelation system at thermal equilibrium with the surrounding is composed of a concentrated polymer-cross-linker solu- tion together with the ice template distributed along the system (Okay & Lozinsky, 2014). Cryogelation leads to the formation of cross-linked polymers even at very low polymer concentrations due to the fact that the effect of the cryoconcentration commonly dominates over the re- duction in the cross-linking rates at low temperatures. After cryogela- tion and melting of ice temple, a 3D polymer network containing macropores is obtained.
Physically cross-linked HA cryogels exhibiting a storage modulus of around 100 Pa were prepared via freeze-thaw induced gelation at a low pH (Cai, Zhang, Wei, & Zhang, 2017). HA cryogels sustaining up to around 30 kPa compressive stresses have also been prepared in an aqueous NaOH solution (pH > 10) of HA at −18 °C using EGDE as a chemical cross-linker (Strom, Larsson, & Okay, 2015). However, the selection of a NaOH solution as the solvent to conduct the cross-linking reactions is not appropriate as it promotes the degradation of HA (Oelschlaeger, Bossler, & Willenbacher, 2016; Tavsanli & Okay, 2016). It seems challenging to produce macroporous HA hydrogels and scaf- folds with appropriate mechanical properties to closely mimic me- chanical properties of the extracellular matrix, structural stability, and an effective mechanism of energy dissipation under strain.
We present here a new cryogelation approach for the fabrication of macroporous HA cryogels with a wide variety of properties, flow-de- pendent viscoelasticity (poroelasticity), complete squeezability, and a high mechanical strength. HA cryogels were synthesized from metha- crylated HA of varying methacrylation degree in aqueous solutions at −18 °C by free-radical mechanism using a redox initiator system. Our preliminary experiments showed that methacrylated HA alone could not form water-insoluble cryogels likely due to the steric effect of HA molecules. However, incorporation of a small amount of a vinyl monomer such as N, N-dimethylacrylamide (DMAA) in the feed resulted in a complete gelation at −18 °C. This reveals spacer effect of PDMAA chains interconnecting HA units, as illustrated in Scheme 1. As will be seen below, HA cryogels in swollen state sustain up to 2.6 ± 0.2MPa compressive stress, which is around 2 orders of magnitude higher than those obtained by EGDE cross-linker (Strom et al., 2015). HA cryogels confined between parallel plates also exhibit reversible strain-depen- dent apparent gel-to-sol transition behavior due to the flowing-out and flowing-in water through the pores, similar to water squeezing out of a sponge. This flow-dependent viscoelasticity of HA cryogels, known as poroelasticity (Hu & Suo, 2012; Nosellia, Lucantonioa, McMeeking, & DeSimonea, 2016; Oyen, 2014), is similar to that observed with ar- ticular cartilage (Lu & Mow, 2008), a low-friction and load bearing soft tissue, providing the joint with vital biomechanical functions, such as wear resistance, load bearing, and shock absorption for around a
century. Under compression, the liquid within the cartilage flows out of the tissue through the pores, as observed in HA cryogels, which pro- duces high frictional resistance and hence frictional energy dissipation responsible for the viscoelastic behavior of articular cartilage (Lu & Mow, 2008). Gel-to-sol transition behavior of HA cryogels presented here is also of great interest in biomaterial and biomedical applications as it protects HA network from damage under large strain conditions and hence acts as a self-defense mechanism.
2. Experimental section
The sodium salt of hyaluronic acid from Streptococcus equi (HA) with a viscosity average molecular weight of ∼1.2× 106 g·mol−1 (Strom et al., 2015), glycidyl methacrylate (GM), N,N-dimethylacrylamide (DMAA), tetrabutylammonium bromide (TBAB), ammonium persulfate (APS), N,N,N',N'-tetramethylethylenediamine (TEMED), all from Sigma- Aldrich, triethylamine (TEA, Merck), and acetone (Tekkim, Turkey), were used as received. A stock solution of APS was prepared by pi- petting 10mL distilled